410 - Energy Alloys, LLC
410 is a martensitic stainless steel that is predominately used in a wide variety wellhead applications. It is a very deep hardening, heat treatable stainless steel that contains Carbon, Manganese, and Chromium as the primary hardening elements. 410 - Rolled Alloys, Inc.410 stainless is a corrosion and heat resistant 12% chromium steel. It is the most widely used of the hardenable stainless steels. Heat treated 410 has mechanical properties comparable to the engineering alloy steel AISI 4130, coupled with the additional benefit of good corrosion resistance. 410 is highly resistant to atmospheric corrosion.
410 Martensitic Stainless Steel Bar | Interlloy | Engineering 410 stainless chemistry Heat treatment
A double tempering treatment as follows is recommended for optimum toughness.Heat to 650 o C - 680 o C. *Soak as required. Cool in air Followed by: Re-heat to 620 o C - 660 o C. *Soak as required. Cool in air. 410 can of course be tempered at much lower temperatures, producing much higher tensile strengths, but with subsequent lower impact properties. NB. 410 STAINLESS STEEL UNS S41000ASTM A479/479M (Chemistry Only) NACE MR0175/ISO 15156 A martensitic stainless which is capable of good wear and corrosion resistance CHEMICAL ANALYSIS RANGE (WT%) C 0.15 Max P 0.040 Max Si 1.00 Max S 0.030 Max Mn 1.00 Max Cr 11.50 13.50 HEAT TREATMENT 410 Stainless Datasheet - upmet 410 stainless chemistry Heat treatmentType 410 is hardenable, straight-chromium stainless steels which combine superior wear resistance of high carbon alloys with the excellent corrosion resistance of chromium stainless steels. Oil quenching these alloys from temperatures between 1800F to 1950F (982-1066C) produces the highest strength and/or wear resistance as well as corrosion resistance. Type 410 alloy is used where strength, hardness, and/or wear resistance must be combined with corrosion resistance.
410 Stainless Steel - Penn Stainless
Alloy 410 contains a minimum of 11.5% chromium which is just sufficient enough to demonstrate corrosion resistance properties in mild atmospheres, steam, and many mild chemical environments. It is a general purpose grade that is often supplied in the hardened but still machineable condition for applications where high strength and moderate heat and corrosion resistance are required. 410 Stainless Steel 410 Stainless Steel Tube - Guanyu Tube410 Stainless Steel Heat Treatment. 410 Stainless Steel Annealing. Full anneal 815-900C, slow furnace cool to 600C and then air cool. Process Anneal 650-760C and air cool. 410 Stainless Steel Hardening. Heat to 925-1010C, followed by quenching in oil or air. Oil quenching is necessary for heavy sections. 410 Stainless Steel Sheet, Bar & Plate - AMS 5504Grade 410 stainless steel is a hardenable, martensitic stainless steel that features a minimum addition of 11.5% chromium. This addition of chromium provides a significant increase in corrosion resistance in mildly corrosive environments where high strength and moderate heat resistance are required.
410 Stainless Steel | Premium Alloys
410 stainless steel is a magnetic 11.5% chromium all-purpose martensitic stainless steel providing favorable corrosion resistance and a broad scope of mechanical properties. The level of resistance can be enhanced by a process of heat treatment and is ideal for jobs requiring good corrosion resistance and high strength. 410 Stainless Steel, UNS S41000Alloy 410 is a martensitic stainless steel that providesmoderate corrosion resistance plus high strength andhardness. This alloy can be hardened by cold working and by heat treating and is magnetic inboth conditions. A wide of properties can be achieved with different heat treatments.. 410 Steel Chemical composition, Metal Properties, Datasheet 410 stainless chemistry Heat treatmentHeat Treatment of steel grade 410. Heat treated : 1472C - 1269C. Technological Curves of steel grade 410
410/420 Stainless Steel Bar - National Specialty Alloys
After heat treatment, Stainless Steel 410 exhibits high mechanical properties, it is magnetic in both hardened and annealed conditions. Upon specification, Stainless Steel 410 can be delivered in a hardened, yet still machinable state for uses where moderate corrosion resistance and high strength are required. AISI 410 Stainless Steel Properties, SS410 Heat Treatment 410 stainless chemistry Heat treatmentAISI 410 stainless steel is one of the most commonly used martensitic stainless steels. It 410 stainless chemistry Heat treatment ATI 410/ATI 420/ATI 425 Mod/ ATI 440A/ATI 440CFor maximum hardness and strength, a hardening heat treatment is necessary. The stainless steel alloys shown in the table above were heated as sheet samples for 60 minutes per inch of thickness at 1800F (982C) for Type ATI 410 and at 1900F (1038C) for ATI 420, ATI 425 Modified, and ATI 440A alloys, and then air cooled to room temperature.
Alloy 410 Martensitic Stainless Steel Plate - Sandmeyer Steel
Alloy 410 (UNS S41000) is a 12% chromium martensitic stainless steel plate that can be heat treated to obtain a wide range of mechanical properties. The alloy has good corrosion resistance along with high strength and hardness. In the annealed condition, 410 stainless steel plate is ductile and may be formed. Confused about Annealing / Heat Treating Terminology 410 stainless chemistry Heat treatmentIn the broadest sense annealing is the process of heating an alloy to an elevated temperature to promote a homogenous chemistry, equiaxed microstructure and uniform mechanical properties to produce what is essentially stress free, or soft material. In the stainless steel, nickel and titanium alloy industries, the terms anneal, solution anneal and solution heat treatment, are used interchangeably. Custom 450 Stainless Steel, UNS S45000A single-step aging treatment develops higher strength with good ductility and toughness. Because it has corrosion resistance similar to alloy 304 stainless and with much higher yield strength, Custom 450 has been used in applications where alloy 304 was not strong enough. It has also replaced alloy 410 stainless